Presentation on theme: "Development of Bialkali Transfer Photocathodes for Large Area Micro- Channel Plate Based Photo Detectors 1 Argonne National Laboratory, Argonne, IL 2 University."— Presentation transcript:
Development of Bialkali Transfer Photocathodes for Large Area Micro- Channel Plate Based Photo Detectors 1 Argonne National Laboratory, Argonne, IL 2 University of Chicago, Chicago, IL 3 Fermi National Accelerator Laboratory, Batavia, IL Junqi Xie 1, Marcel W. Demarteau 1, Henry J. Frisch 1,2, Joe Gregar 1, Richard Northrop 2, Alexander Paramonov 1, Anatoly Ronzhin 3, Greg Sellberg 3, Robert G. Wagner 1, Dean Walters 1, Zikri Yusof 1 On behalf of LAPPD Collaboration
Outline Motivation Small PMT Photocathode Growth and Characterization Large Area Photocathode Growth and Characterization Summary Future Work 2
Motivation: LAPPD Approach 3 61 cm 41 cm PMTLAPPD 3
Incoming photon Glass Window Photocathode MCP1 Anode signal generation MCP2 Many fundamental detector properties such as dark current, quantum efficiency, response time, and lifetime are determined by the properties of the photocathode. Motivation: Photocathode Photocathode: Convertion of photons to electrons 4
Resource: Infrastructure 5 Basic Sciences Program Growth and Characterization Facility General Lab-Infrastructure User facility use APS NSLS Nano center BNL/ANL Basic Sciences Program Growth and Characterization Facility General Lab-Infrastructure User facility use APS NSLS Nano center BNL/ANL Large Area Development Growth Equipment Source Development Infrastructure Large Area Development Growth Equipment Source Development Infrastructure Microscopic Property Macroscopic Property Industrial Fabrication Production Unit (8’’X8’’) (not yet existing) Test Facility for Recipe optimization (industrial standard) Detector integration Facility Production Unit (8’’X8’’) (not yet existing) Test Facility for Recipe optimization (industrial standard) Detector integration Facility
In-Situ Structural and Chemical Characterization In-situ X-ray Scattering (by K. Attenkofer and S. Lee) Macroscopic film properties –Film thickness –Roughness Microscopic composition –Which phases are present –Lateral and transversal and homogenuity –Crystalline size –Preferential crystal growth Surface composition –Local workfunction –Chemical composition Movie like characterization during the growth: An Sb phase transition was observed from amorphous to crystalline at 7~8 nm by XRD. In-situ Sb layer growth and K inter-diffusion process were monitored by real-time XRR. 6
Small PMT Photocathode Growth Process Oxygen discharge cleaning and oxidation; Sb deposition monitoring via reflectivity measurement; Bake out temperature, deposition temperature; Control of alkali metals deposition. Apply these to the fabrication of large area photocathode. 7
Commissioning of Optical Station Movable optical station can be used for both in situ and ex situ optical and electrical measurements. QE measurement by Hamamatsu and ANL optical station agree well with each other indicating the home-built optical station is reliable. 8
Small PMT Photocathode Characterization QE Measurement I-V Characteristic Cathodes exhibit characteristic I-V behavior, with QE as high as 24% at 370 nm. The quick drop at short wavelength is due to glass absorption. 9
The Chalice Design Design is based on the small PMT tube, the chalice can be seen as a LARGE PMT tube. Top glass plate is replaceable for reuse. Chalice structure is supported by external legs. An X-Y scanner was designed and built for QE scan. 10
Sb Beads Arrangements for the Chalice Numerical simulation of Sb thickness as a function of Sb beads arrangements and distance from window; 4 Sb beads arrangement 2.5” distance from the window; This arrangement produces sufficient uniformity on a 4”x4” window as our starting point; This assumes all the beads perform identically. 11
12 Chalice Photocathode Characterization QE Measurement I-V Characteristic Plasma was not performed properly, due to low plasma power supply.
Chalice Photocathode Deposition The QE mapping is obtained at 350 nm wavelength, scan step size: 0.2 inch Sb bead QE Scale The blue area is the 4’’X4’’ window edge. QE is uniform (15%) at a large area. 13
Sb bead Center X: Lighting rod, which affect the Sb film deposition X X Comparison of QE Map and Sb Transmission Map 1 bead 4 beads 14 QE Map Sb Film Transmission Map
Sb Film Transmission Curve with Different Photocathode QE Film transmission with known QE were measured and plotted. Film transmission increases as wavelength increases without regarding the QE value The film transmission values at 400 nm were chosen to plot the relation between KCs-Sb cathode QE and film transmission. The highest QE is around 78% Sb transmission (400nm beam). 15
Summary Photocathode growth and characterization instruments were set up. PMT photocathodes with QE as high as 24% have been produced. Large area (4’’X4’’) photocathode with uniform QE (15%) were achieved even without proper oxygen plasma cleaning and oxidation. All photocathodes show typical I-V characteristics. QE of the photocathode is related to base Sb layer thickness. The optimized Sb thickness for KCs-Sb photocathode is around 78% transmission (400nm beam). 16 Next Steps Work out the plasma configuration to obtain uniform photocathode. Complete absolute reflection measurement of Sb films and relate to the film transmission data. Study the effect of plasma cleaning and oxidation to the photocathode QE. Optimize the process for higher QE cathode based on the micro and macro studies.
Relation between Cathode QE and Sb Film Transmission Relate the QE of the KCs-Sb cathodes with the Sb film transmission at 400 nm. KCs-Sb Photocathode Cs-Sb Photocathode Note that the highest QE is around 78% Sb transmission (400nm beam), similar to that of Cs-Sb cathode at around 82% Sb transmission (blue light) as reported. 18 MARTIN ROME, J. Appl. Phys, 26, 166, 1955
Your consent to our cookies if you continue to use this website.